Book chapter 5

## Introduction to Surface and Thin Film Processes John A. Venables Cambridge University Press (2000)

### Supplementary notes by John A. Venables

© Arizona Board of Regents for Arizona State University and John A. Venables

## Section 5.1: Introduction: growth modes and nucleation barriers

In section 5.1.3 a point of confusion (in the orginal 2000 printing) has been noted by some students about the relation between a) the statement on page 146 starting "When we deposit material A on B, we get layer growth if γA < γB + γ*, where γ* is the interface energy, and vice versa for island growth", and b) the illustrations of figure 5.3(a) and (b) on page 147. This addendum discusses this confusion in more detail so that you can become really confused...

Figure 5.3 derives from my more recent review (Venables 1994, figure 1) where I was wishing to compare compactly both the layer and the SK growth mode in what is here figure 5.3(a). The point here is that layer growth is definitely favored if γA < γB. However if the interface energy builds up as the layers are deposited, then at some stage a switch to islands can occur; this is the SK mode. But figure 5.3(b) illustrates the growth of islands of B on A, not A on B. So in this case the equation on page 146 describes island growth of B on A: γB + γ* > γA; the interest in considering A on B, and then B on A, arises from the role of these two different interfaces in multilayers.

Just to prove that this topic has a jinx on it, there was also an error in the 1994 review text description of what is here figure 5.3(a). But the bottom line is that the statement on page 146 of the original printing was incorrect for describing layer growth of A on B; it should be γA + γ* < γB, and has been corrected in the 2006 printing. Thanks especially to Dr John R. Abelson and his students at UIUC for pointing out this error, and for veryifying this "clarification".